- 273 Views
- Uploaded on
- Presentation posted in: General

ION IMPLANTATION - Chapter 8 Basic Concepts

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

ION IMPLANTATION - Chapter 8

Basic Concepts

• Ion implantation is the dominant method of doping used today. In spite of

creating enormous lattice damage it is favored because:

• Large range of doses - 1011 to 1016 /cm2

• Extremely accurate dose control

• Essential for MOS VT control

• Buried (retrograde) profiles are possible

• Low temperature process

• Wide choice of masking materials

• There are also some

significant disadvantages:

• Damage to crystal.

• Anomalous transiently

enhanced diffusion (TED).

upon annealing this damage.

• Charging of insulating

layers.

A. Implant Profiles

• At its heart ion implantation is a random

process.

• High energy ions (1-1000keV) bombard

the substrate and lose energy through

nuclear collisions and electronic drag forces.

• Profiles can often be described

by a Gaussian distribution, with

a projected range and standard

deviation. (200keV implants

shown.)

(1)

or

(2)

where Q is the dose in ions cm-2 and is

measured by the integrated beam current.

Ranges and standard deviation ∆Rp of dopants in randomly oriented silicon.

• Monte Carlo simulations of the

random trajectories of a group of ions

implanted at a spot on the wafer show

the 3-D spatial distribution of the ions.

(1000 phosphorus ions at 35 keV.)

• Side view (below) shows Rp and ∆Rp

while the beam direction view shows

the lateral straggle.

• The two-dimensional distribution is often assumed to be composed of just the

product of the vertical and lateral distributions.

(3)

• Now consider what happens at a mask edge - if the mask is thick enough to block

the implant, the lateral profile under the mask is determined by the lateral straggle.

(35keV and 120keV As implants at the edge of a poly gate from Alvis et al.)

(Reprinted with permission of J. Vac. Science and Technology.)

• The description of the profile at the mask edge is given by a sum of point

response Gaussian functions, which leads to an error function distribution under

the mask. (See page 7 of class notes on diffusion for a similar analysis.)

B. Masking Implants

• How thick does a mask have to be?

• For masking,

(4)

• Calculating the required mask thickness,

(5)

• The dose that penetrates the mask is given by

(6)

C. Profile Evolution During Annealing

• Comparing Eqn. (1) with the Gaussian

profile from the last set of notes, we see

that ∆Rp is equivalent to . Thus

(7)

• The only other profile we can calculate

analytically is when the implanted

Gaussian is shallow enough that it can

be treated as a delta function and the

subsequent anneal can be treated as a

one-sided Gaussian. (Recall example in

Chapter 7 notes.)

(8)

• Real implanted profiles are more complex.

• Light ions backscatter to skew the profile up.

• Heavy ions scatter deeper.

• 4 moment descriptions of these profiles are

often used (with tabulated values for these

moments).

(9)

Range:

(10)

Std. Dev:

(11)

Skewness:

• Real structures may be even more

complicated because mask edges

or implants are not vertical.

(12)

Kurtosis:

D. Implants in Real Silicon - Channeling

• At least until it is damaged by the

implant, Si is a crystalline material.

• Channeling can produce unexpectedly

deep profiles.

• Screen oxides and tilting/rotating the

wafer can minimize but not eliminate

these effects. (7˚ tilt is common.)

• Sometimes a dual Pearson profile

description is useful.

• Note that the channeling decreases

in the high dose implant (green

curve) because damage blocks the

channels.

Modeling of Range Statistics

• The total energy loss during an ion

trajectory is given by the sum of nuclear

and electronic losses (these can be

treated independently).

(13)

(14)

A. Nuclear Stopping

• An incident ion scatters off the core charge on

an atomic nucleus, modeled to first order by a

screened Coulomb scattering potential.

(15)

• This potential is integrated along the path of the

ion to calculate the scattering angle. (Look-up

tables are often used in practice.)

• Sn(E) in Eqn. (14) can be approximated as shown

below where Z1, m1 = ion and Z2, m2 = substrate.

(16)

B. Non-Local and Local Electronic Stopping

• Drag force caused by charged ion in

"sea" of electrons (non-local electronic

stopping).

• Collisions with electrons around

atoms transfers momentum and

results in local electronic stopping.

(17)

• To first order,

where

C. Total Stopping Power

• The critical energy Ec when the nuclear

and electronic stopping are equal is

B: ≈ 17keV

P: ≈ 150keV

As, Sb : > 500keV

• Thus at high energies, electronic

stopping dominates; at low energy,

nuclear stopping dominates.

Damage Production

• Consider a 30keV arsenic ion, which has

a range of 25 nm, traversing roughly 100

atomic planes.

(18)

• Molecular dynamics simulation of a

5keV Boron ion implanted into silicon

[de la Rubia, LLNL].

• Note that some of the damage anneals

out between 0.5 and 6 psec (point

defects recombining).

Amorphization

• For high enough doses, the crystal becomes amorphous and loses all long range

order. At this point, the arrangement of lattice atoms is random and the damage

accumulation has saturated.

• Cross sectional TEM images of amorphous layer formation with increasing

implant dose (300keV Si -> Si) [Rozgonyi]

• Note that a buried amorphous layer forms first and a substantially higher dose is

needed before the amorphous layer extends all the way to the surface.

• These ideas suggest preamorphizing the substrate with a Si (or Ge) implant to

prevent channeling when dopants are later implanted.

Damage Annealing - Solid Phase Epitaxy

• If the substrate is amorphous,

it can regrow by SPE.

• In the SPE region, all damage

is repaired and dopants are

activated onto substitutional

sites.

• Cross sectional TEM images of

amorphous layer regrowth at

525˚C, from a 200keV, 6e15 cm-2

Sb implant.

• In the tail region, the material is not amorphized.

• Damage beyond the a/c interface can nucleate

stable, secondary defects and cause transient

enhanced diffusion (TED).

Damage Annealing - “+1” Model

Goals: • Remove primary damage created by the implant and activate the dopants.

• Restore silicon lattice to its perfect crystalline state.

• Restore the electron and hole mobility.

• Do this without appreciable dopant redistribution.

• In regions where SPE does not take place

(not amorphized), damage is removed by

point defect recombination.

• Bulk and surface recombination take place

on a short time scale.

• "+1" I excess remains. These

I coalesce into {311} defects

which are stable for longer

periods.

• {311} defects anneal out in sec

to min at moderate temperatures

(800 - 1000˚C) but eject I TED.

Dopant Activation

• When the substrate is amorphous, SPE provides an ideal way of repairing the

damage and activating dopants (except that EOR damage may remain).

• At lower implant doses, activation is much more complex because stable defects

form.

• Plot (above left) of fractional activation versus anneal temperature for boron.

• Reverse annealing (above right) is thought to occur because of a competition

between the native interstitial point defects and the boron atoms for lattice sites.

Transient Enhanced Diffusion

• TED is the result of interstitial damage from

the implant enhancing the dopant diffusion

for a brief transient period.

• It is the dominant effect today that determines

junction depths in shallow profiles.

• It is anomalous diffusion, because profiles can

diffuse more at low temperatures than at high

temperatures for the same Dt.

• The basic model for TED assumes that all the

implant damage recombines rapidly, leaving

only 1 interstitial generated per dopant atom

when the dopant atom occupies a

substitutional site (the +1 model) [Giles].

• TED effects may be very non-local.

• After 900˚C, 1 sec anneal, the amorphous As

surface profile recrystalizes by SPE without

much TED.

• The buried boron layer is drastically affected

by the +1 interstitials in the As tail region.

Atomic Level Understanding Of TED

• {311} clusters form rapidly and then are

stable for extended periods (sec - min),

driving TED by emitting I while they

shrink.

• By 0.1 sec (750˚C), the {311} defects have

formed and CI is down to ≈ 1013 cm-3

(SUPREM).

• But ≈ 108 cm-3 at 750˚C, so the

enhancement is > 105!

• On a much larger time scale, the {311}

clusters decay.

• These act as an ongoing source of excess

interstitials which drives TED.

• TED lasts hours at very low T, minutes

at intermediate T and msec at very high T.

• Given this picture, we can model the

{311} behavior as follows:

(where Cln is a cluster with n interstitials)

(19)

(20)

• The most important part of the transient is while the {311} clusters are evaporating

I, maintaining a constant supersaturation of I.

• During this period, dopant diffusivity enhancements are ≈ constant and given

by (see text):

(21)

• Note that the diffusivity enhancement is as

large as 10,000 at low T and falls off to 100 -

1000 at RTA temperatures.

• These calculated values agree with

experimental measurements.

Estimating the Duration of TED

• Over time the interstitial supersaturation

decays to zero and TED ends.

• Example - Boron TED (TSUPREM IV).

Note that CI/has dropped from 104 to

102 in 10 min at 750˚C.

• The excess I diffuse into the bulk and

recombine at the surface.

• Note the relatively flat interstitial

profiles (dashed) except at the surface

where recombination is occurring.

• The flux towards the surface is

where RP is the range of the implant.

• The time to dissolve the clusters is given

by the dose divided by the flux (see text):

(22)

• Plot of Eqn. 22. This matches the experimental

data on page 18 of these notes (Fig. 8-33 in text).

• Note that TED persists for hours at low T and

disappears in msec at very high T.

• Thus the general picture of TED that emerges is

as shown on the lower left.

• Because the {311} clusters exist for much longer

times at low T, there can actually be greater

dopant motion during low T anneals (below).

• 2D SUPREM simulation of small MOS

transistor.

• Ion implantation in the S/D regions

generates excess I. These diffuse into the

channel region pushing boron (channel

dopant) up towards the surface.

• Effect is more pronounced in smaller

devices.

• Result is that VTH depends on

channel length (the "reverse short

channel effect" only recently

understood).

(See text - Chpt. 7 - for more details on this example.)

Summary of Key Ideas

• Ion implantation provides great flexibility and excellent control of implanted

dopants.

• Since implanted ion energies are >> Si-Si binding energy (≈ 15 eV), many Si

lattice atoms are displaced from lattice positions by incoming ions.

• This damage accumulates with implanted dose and can completely amorphize

the substrate at high doses.

• The open structure of the silicon lattice leads to ion channeling and complex

as-implanted profiles.

• TED is the biggest single problem with ion implantation because it leads to

huge enhancements in dopant diffusivity.

• Understanding of TED has led to methods to control it (RTA annealing).

• Nevertheless, achieving the shallow junctions required by the NTRS will be a

challenge in the future since ion implantation appears to be the technology

choice.